Download presentation

Presentation is loading. Please wait.

Published byGrayson Cartledge Modified about 1 year ago

1

2
NCAT1 Aggregate Properties HMA

3
NCAT2 To be Covered Specific Gravities Consensus Properties

4
NCAT3 All matter has mass and occupies space. Volumetrics are the relationships between mass and volume Superpave mix design based on aggregate and mixture volumetrics Volumetrics

5
NCAT4 Specific Gravity, G Ratio of the mass to volume of an object to that of water at the same temperature Mass Solid Volume Mass Water Volume

6
NCAT5 Densities Density is the unit weight of a material –lb/ft 3 or kg/m 3 –Unit weight = w G w = g/cm 3 w = 1000 kg/m 3 w = 62.4 lb/ft 3 l Bulk density means sample contains more than one mass and/or volume

7
NCAT6 G sb = Mass, oven dry Bulk Specific Gravity, Dry Vol of agg, + surface voids Vol. of water-perm. voids Surface Voids

8
NCAT7 G s, ssd = Mass, oven dry agg + mass water Bulk Specific Gravity, SSD Vol of agg, + surface voids Vol. of water-perm. voids Surface Voids

9
NCAT8 G sa = Mass, oven dry agg Bulk Specific Gravity, Apparent Vol of agg

10
NCAT9 Phase Diagram Phase: a change in state (e.g. solid, liquid, gas) Mass (Weight) Volume V = (mass) / (G s w ) Water permeable voids Aggregate Solids

11
NCAT10 Specific Gravity Tests for Aggregates Two tests are needed –Coarse aggregate (retained on the 4.75 mm sieve) –Fine aggregate (passing the 4.75 mm sieve)

12
NCAT11 Coarse Aggregate Specific Gravity ASTM C127 –Dry aggregate –Soak in water for 24 hours –Decant water –Use pre-dampened towel to get SSD condition –Determine mass of SSD aggregate in bucket –Determine mass under water –Dry to constant mass –Determine oven dry mass

13
NCAT12 Coarse Aggregate Specific Gravity

14
NCAT13 Coarse Aggregate Specific Gravity

15
NCAT14 Coarse Aggregate Specific Gravity Calculations G sb = A / (B - C) –A = mass oven dry –B = mass SSD –C = mass under water G s,SSD = B / (B - C) G sa = A / (A - C) Water absorption capacity, % –Absorption % = [(B - A) / A] * 100

16
NCAT15 Fine Aggregate Specific Gravity ASTM C128 –Dry aggregate –Soak in water for 24 hours –Spread out and dry to SSD –Add 500 g of SSD aggregate to pycnometer of known volume Pre-filled with some water –Add more water and agitate until air bubble have been removed –Fill to line and determine the mass of the pycnometer, aggregate and water –Empty aggregate into pan and dry to constant mass –Determine oven dry mass

17
NCAT16 Fine Aggregate Specific Gravity

18
NCAT17 Fine Aggregate Specific Gravity

19
NCAT18 Fine Aggregate Specific Gravity

20
NCAT19 Fine Aggregate Specific Gravity Calculations G sb = A / (B + S - C) –A = mass oven dry –B = mass of pycnometer filled with water –C = mass pycnometer, SSD aggregate and water –S = mass SSD aggregate G s,SSD = S / (B + S - C) G sa = A / (B + A - C) Water absorption capacity, % –Absorption % = [(S - A) / A] * 100

21
NCAT20 Concensus Aggregate Properties Coarse Aggregate Particle Shape % Crushed Faces Flat and Elongated Fine Aggregate Particle Shape Clay Content ** Determined for the blended aggregate gradation **

22
NCAT21 Percent Crushed Fragments in Gravels Quarried materials always 100% crushed Minimum values depended upon traffic level and layer (lift) Defined as % mass with one or more fractured faces

23
NCAT22 Percent Crushed Fragments in Gravels 0% Crushed 100% with 2 or More Crushed Faces

24
NCAT23 Coarse Aggregate Angularity Criteria TrafficDepth from Surface Millions of ESALs 100 mm < 0.3 < 1 < 3 < 10 < 30 < 100 /-- 65/-- 75/-- 85/80 95/90 100/100 --/-- 50/-- 60/-- 80/75 95/90 100/100 First number denotes % with one or more fractured faces Second number denotes % with two or more fractured faces

25
NCAT24 Flat and Elongated Particles ASTM D4791 –Flat –Elongated –Total flat and elongated Superpave –Flat and Elongated –Maximum to minimum dimension 5:1 3:1 2:1

26
NCAT25 Flat and Elongated Maximum Minimum

27
NCAT26 Flat and Elongated Maximum Minimum

28
NCAT27 Flat and Elongated Criteria TrafficMaximum, Percent Millions of ESALs < 0.3 < 1 < 3 < 10 < 30 < 100

29
NCAT28 Fine Aggregate Angularity (Uncompacted Void Content of Fine Aggregate) * Fine aggregate at a specified gradation is allowed to flow freely into a 100 cm 3 cylinder. *Knowing the specific gravity of the aggregate, the voids between aggregate particles can be determined * The more angular the aggregate, the higher the void content

30
NCAT29 Fine Aggregate Angularity Natural sands: typically < 45 Manufactured sands: typically > 42

31
NCAT30 Fine Aggregate Angularity Criteria TrafficDepth from Surface Millions of ESALs 100mm < 0.3 < 1 < 3 < 10 < 30 < 100

32
NCAT31 Clay Content (Sand Equivalent Test) * ASHTO T176, ASTM D Used to estimate the relative proportions of fine agg. and clay-like or plastic fines and dust. SE = Sand Reading Clay Reading Sand Reading Clay Reading Flocculating Solution Suspended Clay Sedimented Aggregate *100

33
NCAT32 Bottle of Solution on Shelf Above Top of Cylinder Hose and Irrigation Tube Measurement Rod

34
NCAT33 Marker on Measurement Rod Top of Suspended Material Top of Sand Layer

35
NCAT34 Clay Content Criteria TrafficSand Equivalent Millions of ESALs Minimum, Percent < 0.3 < 1 < 3 < 10 < 30 < 100

36
NCAT35 Questions - ?

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google